Реклама

Current Applied Physics 16 (2016) 931e938 Contents lists available at ScienceDirect Current Applied Physics journal homepage: www.elsevier.com/locate/cap Peculiarities in the pseudogap behavior in optimally doped YBa2Cu3O7d single crystals under pressure up to 1 GPa A.L. Solovjov a, b, L.V. Omelchenko a, b, R.V. Vovk c, O.V. Dobrovolskiy c, d, *, S.N. Kamchatnaya c, D.M. Sergeev e a B. I. Verkin Institute for Low Temperature Physics and Engineering, 61103, Kharkiv, Ukraine International Laboratory of High Magnetic Fields and Low Temperatures, 53421, Wroclaw, Poland Physics Department, V. Karazin Kharkiv National University, Svobody Sq. 4, 61077, Kharkiv, Ukraine d Physikalisches Institut, Goethe University, Max-von-Laue-Str. 1, 60438, Frankfurt am Main, Germany e Zhubanov Aktobe Regional State University, 030000, Aktobe, Kazakhstan b c a r t i c l e i n f o a b s t r a c t Article history: Received 16 March 2016 Received in revised form 11 May 2016 Accepted 18 May 2016 Available online 20 May 2016 The inﬂuence of the hydrostatic pressure P up to 0.95 GPa on the excess conductivity s0 (T) and the pseudogap D*(T) in optimally doped YBa2Cu3O7d single crystals (Tc x 91.1 K at ambient pressure) is investigated by electrical resistivity measurements. A pronounced enhancement of the pseudogap under pressure of dlnD*/dP z 0.32, which is only a factor of 1.12 smaller than in slightly doped single crystals, is revealed for the ﬁrst time. This implies a somewhat more moderate increase of the coupling strength in optimally doped cuprates with increasing pressure. Simultaneously, the ratio 2D*(Tc)/kBTc z 5 at P ¼ 0 GPa, which is typical for high-temperature superconductors with strong coupling, increases by 16% with increasing pressure. At the same time, the pressure effect on Tc is minor: dTc/dP z þ0.73 K GPa1, whereas dlnr/dP z (17 ± 0.2)% GPa1 is comparable with that in lightly doped YBCO single crystals. This suggests that the mechanisms of the pressure effect on r(T) and Tc are noticeably different. Independently of pressure, near Tc, s0 (T) is well described by the Aslamazov-Larkin (3D-AL) and 2D HikamiLarkin ﬂuctuation theories, exhibiting a 3De2D crossover with increasing temperature. However, the temperature interval Tc < T < T01, in which s0 (T) obeys the classical ﬂuctuation theories, is exceptionally narrow (z1.16 K). Nevertheless, a peculiarity at the temperature T01, up to which the wave function phase stiffness in the superconductor is maintained, is clearly observed in the dependence D*(T). Below T01 a fast growth of D*(T) is revealed for the ﬁrst time. It can be associated with a sudden increase of the superﬂuid density, ns, that is the density of ﬂuctuating Cooper pairs (short-range phase correlations) forming in the sample when T approaches Tc. © 2016 Elsevier B.V. All rights reserved. Keywords: Superconducting cuprates Pseudogap Pressure Electrical resistance measurements 1. Introduction In addition to a high critical temperature, Tc [1], hightemperature superconductors (HTSCs) with active CuO2 planes (cuprates) possess a series of other unconventional properties [2e6]. Among these are a low density of the charge carriers, nf, which even in optimally doped samples is by an order of magnitude smaller than in conventional metals [6], strong electron correlations [7], quasi-two-dimensionality caused by the conductivity within the CuO2 planes [8], and, in consequence of this, a strong * Corresponding author. Physikalisches Institut, Goethe University, Max-vonLaue-Str. 1, 60438, Frankfurt am Main, Germany. E-mail address: Dobrovolskiy@Physik.uni-frankfurt.de (O.V. Dobrovolskiy). http://dx.doi.org/10.1016/j.cap.2016.05.014 1567-1739/© 2016 Elsevier B.V. All rights reserved. anisotropy of the electronic properties [5e7,9]. One of the most intriguing properties of cuprates is the pseudogap (PG) [5,9e12] which is opening at some characteristic temperature T* [ Tc. By deﬁnition, PG is a state of matter characterized by a reduced (but nonzero) density of electronic states (DOS) at the Fermi level [13]. It should be stressed that the fundamental difference of the PG state from the superconducting (SC) one is that in the latter the SC gap is opening and DOS is equal to zero [9,11]. It is expected that the correct understanding of the PG nature will allow one to shed light on the SC pairing mechanism in HTSCs which remains debatable so far. In particular, this is important for searching for novel superconductors with yet higher Tc’s. The number of theoretical models describing PG is exceptionally large [9,11,12,14e16]. However, no ultimate elucidation of the PG nature 932 A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 is available so far. The majority of theorists assume that PG appears in consequence of ﬂuctuations [17,18]. However, so far there is no generally accepted viewpoint concerning the nature of these ﬂuctuations (see Refs. [10,12] and references therein). Some researchers believe that the appearance of PG is not directly associated with superconductivity [7,10,14e16,19]. As possible sources for the appearance of PG, non-related to superconductivity, are considered such types of interaction as spin ﬂuctuations [7,20], charge-density waves [14], antiferromagnetic spin correlations [19], excitons [21], and polarons [22]. At the same time, the abundance of models points to that a generally accepted viewpoint in this regard is still absent. The role of the electron-phonon interaction (EPI) in the formation of superconducting Cooper pairs at such high temperatures as well as of paired fermions (local pairs) above Tc also remains unclear [23e25]. It is assumed that EPI should take place in cuprates [23], whereby EPI is probably enhanced by some additional interaction of, most likely, magnetic character [10,15,25]. However, recent calculations suggest [24] that the speciﬁc character of EPI in HTS’s stipulates a strong correlational narrowing of the electron Wband. This leads to that the chemical potential m ~ W ≪ J, where J is the electron exchange interaction constant. The fulﬁllment of this condition is crucial for the formation of singlet electron pairs in HTSCs, coupled by a strong effective kinematic ﬁeld. At the same time, the available experimental data do not sufﬁce [25,26] to examine the calculation results. We adhere the viewpoint that PG in cuprates is caused by some speciﬁc ﬂuctuations which lead to the formation of local pairs (LPs) at Tc T T*, preceding the transition to the SC state [3,9,27e31]. According to theory [32e34], at high temperatures T T* LPs appear in the form of strongly bound bosons (SBBs) obeying the Bose-Einstein condensation (BEC) theory. The SBB size is deﬁned by the coherence length in the ab-plane, xab(T) ¼ xab(0)(T/Tc 1)1/2, whose spatial extent xab(0) ~ xab(T*) is exceptionally small. Thus, for YBCO ﬁlms with a close-to-optimal doping level xab(0) ~ 10 Å, typically [35,36]. Accordingly, the coupling strength in such a pair, εb ðx2ab Þ1 is in turn exceptionally strong [32,33]. Such a strong coupling, which can be caused by either of the above-mentioned interaction mechanisms and which is rigid against thermal ﬂuctuations, ensures the possibility of the SBBs formation at such high temperatures. In consequence of this, SBBs are strongly coupled but local, i.e., non-interacting formations, since the pair size is much less than the distance between them. It should be noted that according to theory, SBBs can only appear in systems with a reduced nf. This is, in particular, the case in cuprates with a doping level less than the optimal one. Importantly, PG is observed in HTSCs with just the mentioned doping level. According to theory, LPs appear at some high temperature T* but they can only condensate at Tc ≪ T* [32,33]. This occurs in consequence of Gaussian ﬂuctuations of the order parameter in two-dimensional (2D) systems to which HTSCs belong in a broad temperature range. Such ﬂuctuations hinder the appearance of the phase coherence in the 2D state. As a result, Tc in an ideal 2D metal turns out zero (Mermin-Wagner-Hohenberg theorem), and a ﬁnite value of Tc can only be obtained when three-dimensional effects are taken into account [32,37]. This is why, as our investigations of the ﬂuctuation conductivity (FC) revealed [4,9], HTSCs are always trimerizing when T approaches Tc. At this conjuncture, FC is always described by the standard equation of the classical AslamazovLarkin theory [38] for 3D systems. However, by deﬁnition, noninteracting SBBs cannot condensate at all. This is why the theory [32,38,39] assumes that with decreasing temperature and simultaneously increasing xab(T) SBBs should turn into ﬂuctuational Cooper pairs (FCPs) obeying the BCS theory [40], i.e., it predicts the BEC-BCS crossover [32,37]. The crossover temperature, Tpair, is clearly observed in a series of experiments [4,41]. However, the crossover details are not completely clear so far. Since the discovery of a strong dependence of Tc on pressure in the compound LaeBaeCueO [42], pressure has been playing a rather noticeable role in investigations of HTSCs [43e46]. In contrast to conventional superconductors, the dependence dTc/dP in cuprates in the vast majority of cases is positive, whereas the derivative dlnr/dT is negative and rather large [44e46]. Here r ≡ rab is the resistivity in the ab-plane of the sample, that is parallel to the CuO2 planes. Upon application of pressure the volume of the elementary crystal cell is reduced. This has to contribute to the ordering of the system and should lead to a decrease of the number of structural defects and, hence, to a likely reduction of r. Nevertheless, the mechanisms of the pressure effect on r still remain incomprehensible, since the nature of the transport properties of HTSCs is, strictly speaking, unclear. As is known, the major contribution to the conductivity in cuprates is provided by the CuO2 planes, between which a relatively weak interplane interaction takes place. The application of pressure most likely leads to a rearrangement of the charge carriers resulting in an increase of the charge carriers density nf in the conducting CuO2 planes and, hence, to a reduction of r. Apparently, an increase of nf under pressure should also lead to an increase of Tc [6,9], i.e., to a positive value of dTc/dP, as observed in experiments. Another mechanism, which can also raise Tc, refers to the possible increase of the pairing interaction Veff which has to depend on pressure. For underdoped cuprates the former mechanism is believed to dominate the pressure effect on Tc (see Ref. [26] and references therein). It is well known that in YBCO the unique proximity between the d-Cu state and the p-O state is realized [47,48]. As a result, the band structure of cuprate HTSCs is determined by the strongly correlated electron motion on the Cu(3d) orbital interacting with the O(2p) one. The applied hydrostatic pressure is very likely to affect this interaction. The effect of hydrostatic pressure on rab in HTSCs was experimentally investigated in Ref. [44]. There is also a few works addressing the inﬂuence of pressure on FC in various cuprates [45,46,49,50]. However, apart of a minor number of reports [51e53], there has been very few work devoted to the study of pressure on PG in HTSCs. Here, we investigate the effect of the hydrostatic pressure P z 1 GPa (1 GPa ¼ 10 kbar) on the temperature dependence of the resistivity rab(T) in optimally doped YBa2Cu3O7d single crystals with Tc ¼ 91.07 K at P ¼ 0 GPa. We study the ﬂuctuational contributions to the conductivity, focusing chieﬂy on the temperature dependence of the excess conductivity s0 (T). From an analysis of the excess conductivity we obtain the PG temperature dependence D*(T) at P ¼ 0 GPa as well as at 0.25 GPa, 0.65 GPa, and 0.95 GPa. The analysis is performed in the framework of the local pair model (LP model) [4,9], as detailed in the text. The reported comparison of our results with analogous ones for Bi2 Sr2 CaCu2O8d (BISCCO-2212) [45], HgBa2Ca2Cu3O8 (Hg-2223) [49], HoBa2Cu3O7d (HoBCO) [52] and slightly doped YBa2Cu3O7d single crystals [26,53] should contribute to a better understanding of the inﬂuence mechanisms of pressure on Tc, rab(T), and D*(T) in HTSCs. 2. Experiment YBa2Cu3O7d single crystals (YBCO) were grown by the solutionmelt technique as described elsewhere [54e57]. For resistive measurements crystals of a rectangular shape with the typical sizes 3 0.5 0.03 mm3 were selected. The minimal crystal size corresponds to the c-axis. To obtain samples with a desired oxygen content, the crystals were annealed as detailed in Refs. [55e57]. The electrical resistance in the ab-plane was measured in the standard four-probe geometry [57]. The measurements were done A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 933 in the temperature-sweep mode, with a rate of 0.1 K/min for measurements near Tc and about 5 K/min for T [ Tc. The hydrostatic pressure was created in a chamber of the cylinder-piston type [55,56]. To exclude the inﬂuence of the oxygen redistribution, the measurements were done in twoeseven days after the relaxation processes had been completed [52]. 3. Results and discussion 3.1. Resistivity temperature dependence The temperature dependences of the resistivity r(T) ¼ rab(T) of the YBa2Cu3O7d single crystal with Tc ¼ 91.07 K (P¼0 GPa) and the oxygen index 7 d z 6.94 are shown in Fig. 1 at P ¼ 0 GPa (curve 1) and P ¼ 0.95 GPa (curve 2). The resistivity curves obtained for P ¼ 0.25 GPa and 0.65 GPa are in between these two curves and not shown for the sake of data readability. The shape of the r(T) curve1YBCO ﬁlms [58,59] and single crystals [1,60]. The transition temperature Tc was determined by extrapolating the resistive transition to the value r(Tc) ¼ 0 [61]. In the broad temperature range from 300 K to T* ¼ (141 ± 0.3) K (P ¼ 0 GPa) and T* ¼ (135.7 ± 0.3) K (P ¼ 0.95 GPa) the dependence r(T) is linear with the slope dr/dT ¼ 0.63 mU cm K1 and dr/dT ¼ 0.54 mU cm K1 at P ¼ 0 GPa and P ¼ 0.95 GPa, respectively. It should be noted that as it follows from the theory and experiment [1,6,8,9], in this case the values of the characteristic temperature T* are much smaller than T* x 250 K observed in slightly doped YBCO ﬁlms [9,58,59] and single crystals [53,60]. In addition to this, Tc’s are very high while the resistive transitions are exceptionally sharp, namely DTc ¼ Tc ð0:9r’N Þ Tc ð0:1r’N Þ ¼ 91:2 K 91:07 K ¼ 0:13 K ðP ¼ 0 GPaÞ and DTc ¼ 92 K 91:76 K ¼ 0:24 K ðP ¼ 0:95 GPaÞ. Here, r’N is the resistivity at T ¼ Tons corresponding to the onset of the SC transition [53]. Nevertheless, as in the case of slightly doped single crystals [53], pressure broadens the resistive transition by about a factor of two. The applied pressure usually increases Tc (dTc/dP x þ4 K GPa1) and reduces r(T) (dlnr/dP x 12% GPa1) of cuprates [44e46,52]. In addition to this, it enhances the value of the SC gap, D(0), and the ratio 2D/kBTc [25,26], most likely due to a decrease of the phonon frequencies in cuprates under pressure [25]. In the case studied by us the pressure effect on Tc is very weak: dTc/dP x þ0.73 K GPa1, see also Fig. 2. This is the ﬁrst unexpected result revealed for optimally Fig. 2. Temperature dependences of s0 2(T) of the YBa2Cu3O6.94 single crystal at (a) P ¼ 0 and (b) P ¼ 0.95 GPa. Straight lines are guides for the eye. doped (OD) YBCO single crystals. For comparison, in slightly doped YBCO single crystals with Tc ¼ 49.2 K we observed dTc/ dP x þ5 K GPa1, in good agreement with the above-mentioned average value obtained for YBCO compounds with a relatively close-to-optimal doping level. However, as before, pressure strongly reduces the resistivity of the sample: dlnr/ dP z (17 ± 0.2)% GPa1 that is even greater than the value obtained for Y123 [44] and of the same order of magnitude as reported for Bi2212 in the same reference. Hence, we can conclude that the mechanisms of the pressure effect on Tc and r are different. In optimally doped single crystals the charge carrier density in the CuO2 planes, nf, is maximal. Moreover, it is likely to saturate in YBCO compounds at the oxygen index (7 d z 6.94) we are dealing with in the studied sample. For this reason the pressure has practically no effect on nf as well as on Tc related to it. Hence, we can conclude that the decrease of r(P) is not related to the reduction of nf but it is likely to occur as a result of both, the reduction of the number of structural defects [44] and softening of the phonon spectrum [25] with increasing pressure. Also, we have to emphasize that for our slightly doped YBCO single crystal we observe dlnr/ dP z (19 ± 0.2)% GPa1 which is by 12% larger than that found for the optimally doped one. The ﬁnding is conﬁrmed by the PG results as will be shown below. This fact suggests a slightly weaker inﬂuence of the pressure on the YBCO phonon spectrum in the case of the OD samples. 3.2. Fluctuation conductivity Fig. 1. Resistivity temperature dependences of the optimally doped YBa2Cu3O7d (7 d z 6.94) single crystal at P ¼ 0 GPa (curve 1) and P ¼ 0.95 GPa (curve 2). Dashed lines designate rN(T) extrapolated to the low-temperature region. Inset: Determination of T*. According to the theoretical model of nearly antiferromagnetic Fermi liquid (NAFL) [20], the linear dependence r(T) at high temperatures corresponds to the normal state of the system. This state is characterized by the constancy of various possible interactions in HTSC and, hence, by the stability of the Fermi surface [10,11,20]. Below T*, the measured r(T) curve deviates from the linear dependence towards smaller values. This leads to the appearance of the excess conductivity 934 A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 s’ ðTÞ ¼ sðTÞ s’N ðTÞ ¼ ½1=rðTÞ ½1=rN ðTÞ; s’ ¼ ½rN ðTÞ rðTÞ=½rðTÞrN ðTÞ; (1) where rN(T) ¼ aT þ b is the linear temperature dependence of the sample in the normal state [6,8,20]. By extrapolating rN(T) towards low temperatures and using equation (1), the temperature dependence s0 (T) was determined. Using the LP model [4,9], from the excess conductivity the data for FC and PG in the sample at pressures P ¼ 0 GPa, 0.25 GPa, 0.65 GPa, and 0.95 GPa were deduced. Below we compare the results obtained for P ¼ 0 GPa and P ¼ 0.95 GPa applied during a week. The parameters obtained from the analysis for all samples studied are summarized in Table 1. The ﬁrst step in the LP model analysis requires to deduce the dependence lns0 (lnε) shown in Fig. 3, which determines the range of superconducting ﬂuctuations in the vicinity of Tc [9,38,39]. Here, mf mf ε ¼ ðT=Tc 1Þ is the reduced temperature and Tc is the critical temperature in the mean-ﬁeld approximation [32,62,63], which separates the range of SC ﬂuctuations from the range of critical ﬂuctuations near Tc (where D < kBT), not accounted for within the Ginzburg-Landau theory [64,65]. For the determination of Tcmf one uses the experimental fact that in all HTSCs near Tc, s0 (T) is always extrapolated by the 3D Aslamazov-Larkin (AL) equation [see equation (2) below] [9,35,36,58,59,61]. In this equation s0 (T) diverges as ε1/2 when the temperature is close to Tcmf . Accordingly, s’2 ε ðT Tcmf Þ [66], that allows one to determine Tcmf and, hence, ε. In Fig. 2 we present the dependence s0 2(T) of the investigated sample at P ¼ 0 GPa (panel (a), full circles) and P ¼ 0.95 GPa (panel (b), open squares). The intersection of the linear dependence s0 2(T) with the temperature axis yields Tcmf ¼ 91:08 K > Tc ¼ 91.07 K (P ¼ 0 GPa) and Tcmf ¼ 91:83 K > Tc ¼ 91.76 K (P ¼ 0.95 GPa), respectively. In addition to this, in Fig. 2 we mark the 3D-2D (AL-MT) crossover temperature T0 and the Ginzburg temperature TG, up to which the experimental data obey the AL theory when T approaches Tcmf [67,68]. In Fig. 3 this temperature corresponds to the marked value of ln(εG). The dependence lns0 (lnε) is displayed in Fig. 3 for P ¼ 0 GPa (panel (a), full circles) and P ¼ 0.95 GPa (panel (b), open squares). Both curves are noticeably shifted to the left as compared to the slightly doped YBCO single crystals (Tc ¼ 49.2 K at P ¼ 0 GPa) [53]. This points to the smallness of the coherence length xðTÞ ¼ xð0ÞðT=Tcmf 1Þ1=2 [63] in the sample. Nevertheless, up to T0 z 91.15 K (lnε0 z 7.11, P ¼ 0 GPa) the experimental data are ﬁtted well to the AL ﬂuctuation contribution for 3D systems [38]. s’AL3D ¼ C3D e2 ε1=2 : 32Zxc ð0Þ (2) which is presented by the dashed straight line with the slope l ¼ 1/2 in Fig. 3, and above T0 up to T01 z 92.54 K (lnε01 z 4.2) by the Maki-Thomson (MT) contribution of the Hikami-Larkin (HL) theory [39]. Fig. 3. lns0 vs lnε of the YBa2Cu3O6.94 single crystal at P ¼ 0 GPa (panel a, dots) and P ¼ 0.95 GPa (panel b, open squares) compared with the ﬂuctuation theories: 3D AL (dashed lines 1) and 2D MT (solid curves 2). lnε01 corresponds to T01 which determines the range of SC ﬂuctuations, lnε0 corresponds to the crossover temperature T0, and lnεG designates the Ginzburg temperature TG. s’MT ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ! e2 1 1 þ a þ 1 þ 2a 1 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ε ; ln ðd=aÞ 8dZ 1 a=d 1 þ d þ 1 þ 2d (3) see the solid curve in Fig. 3(a). Analogous results have been obtained for all other pressures, including P ¼ 0.95 GPa, refer to Fig. 3(b), for which T0 z 91.93 K (lnε0 z 6.72) and T01 z 93.18 K (lnε01 z 4.2). As usually, in equations (2) and (3) a ¼ 2[xc(0)/d]2ε1 is the pairing parameter, d¼b 16 xc ð0Þ 2 kB T t4 pZ d (4) is the depairing parameter, and t4 is the ﬂuctuating Cooper pairs relaxation time deﬁned as t4bT ¼ (pZ)/(8kBε01) ¼ A/ε01. Here, b ¼ 1.203(l/xab), where l is the mean free path and xab is the coherence length in the ab-plane in the clean-limit approximation [9]. At T < T0, that is near Tc, the coherence length along the c-axis xc(T) > d, where d ¼ 11.67 Å is the lattice parameter along the c-axis. Accordingly, FCPs can interact in the entire volume of the superconductor, thereby forming the 3D state. That is, HTSCs are always trimerized near the SC transition, in accordance with theory [32e34,37]. Above T0, d > xc(T) > d01, where d01 is the distance between the conducting CuO2 planes. This means that the 3D state is lost, but the Josephson interaction still couples the neighboring CuO2 planes [8,39,69]. Hence, this is a quasi-two-dimensional state of the system, which is described by the 2D-MT ﬂuctuation contribution of the HL theory by equation (3). Consequently, T0 is the MT-AL transition temperature and, simultaneously, the 2D-3D Table 1 Parameters of the optimally doped YBa2Cu3O6.94 single crystal. P GPa r(280 K), mU cm Tc, K Tcmf , K T01, K TG , K DTﬂ, K d1, Å xc(0), Å T*, K Tpair, K D*(TG), K 2D*/kBTc εc0 a0 0 0.25 0.65 0.95 184.6 175.9 168.2 157.3 91.07 91.12 91.51 91.76 91.08 91.3 91.58 91.83 92.54 92.6 92.9 93.18 91.09 91.3 91.6 91.84 1.45 1.3 1.3 1.34 2.72 2.73 3.34 3.3 0.334 0.335 0.47 0.405 141 135 140 135.7 129 127 126 122 228 239 230 273 5 5.2 5.4 5.8 0.154 0.151 0.143 0.147 0.53 0.53 0.54 0.53 A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 crossover temperature. Evidently, xc(T0) ¼ d, that allows one to deduce pﬃﬃﬃﬃﬃ xc ð0Þ ¼ d ε0 : (5) 1 At P ¼ 0 GPa equation (5) yields xc(0) ¼ (3.34 ± 0.02) 10 Å that is very small. One can see in Fig. 3(b) that in this case pressure affects the value of s0 (T) only slightly. Nevertheless, at P ¼ 0.95 GPa xc(0) ¼ (4.05 ± 0.02) 101 Å, i.e., the coherence length slightly grows under pressure, as in other cuprates [49]. Usually, in cuprates the coherence length in the ab-plane, which determines the Cooper pair size, xab(0) ~ 15xc(0). Hence, in our optimally doped single crystal with Tc ~ 91 K xab(0) z 5 Å at P ¼ 0 GPa is expected and this value is in good agreement with our ﬁnding. For comparison, xab(0) is about 13 Å in slightly under-doped YBCO with Tc ¼ 87.4 K [9,35,36,58,59]. In this way, we have got the second nontrivial result, namely a very small pair size at high temperatures where LPs should exist in the form of SBBs. At the same time, as mentioned before, the smaller xab(0), the larger the bound energy in the pair εb ðx2ab Þ1 [32,33,62]. This estimate appears reasonable taking into account the very high Tc of the investigated crystal. Another characteristic temperature in Fig. 3 is T01. It determines the range of the SC ﬂuctuations above Tc. Having determined lnε01 from the data one gets T01 z 92.54 K (lnε01 z 4.2 at P ¼ 0 GPa) and T01 z 93.2 K (lnε01 z 4.2 at P ¼ 0.95 GPa). As mentioned above, at T0 < T < T01, xc(T) < d, but simultaneously xc(T) > d01, that is the system is in the quasi-2D state and it is described by equation (3) [39,69]. Accordingly, above T01, where xc(T) < d01, the pairs are located within the CuO2 planes and do not interact. This is why above T01 the ﬂuctuation theories do not describe the experiment, as is clearly seen in Fig. 3. In this way, it follows that xc(T01) ¼ d01 at T ¼ T01. It is evident that xc(0) ¼ const at a given pressure, so that the pﬃﬃﬃﬃﬃﬃﬃ should be fulﬁlled. Since condition xc ð0Þ ¼ d01 ε01 1 xc(0) ¼ 3.34 10 Å is determined by the temperature of the dimensional crossover T0, see equation (5), this allows one to espﬃﬃﬃﬃﬃﬃﬃ timate d01 ¼ xc ð0Þð ε01 Þ1 . This yields d01 z 2.8 Å at P ¼ 0 GPa and d01 z 3.3 Å at P ¼ 0.95 GPa that is close to the values of d01 determined from structural studies of YBCO [1,70]. In this way, despite the very small values of xc(0), the analysis of the excess conductivity in the framework of the LP model allows one to get reasonable values of d01. However, in contradistinction to lightly doped YBCO single crystals [53], d01 grows slightly with pressure. This may be caused by the error in the determination of lnε01 in Fig. 3 or by the peculiarities in the behavior of optimally doped single crystals under pressure. On the other hand, according to theory [27], it is this temperature T01 up to which the order parameter phase stiffness is maintained in HTSCs, as conﬁrmed in experiments [71]. This means that in the temperature range from Tc to T01 Cooper pairs chieﬂy behave as superconducting pairs. This leads to a behavior of the cuprates, which is unconventional from the viewpoint of “classical” superconductivity. As it was shown in a series of works [3,28,70], the SC gap in HTSCs does not vanish at Tc and the range of SC ﬂuctuations is maintained up to ~120 K in YBCO (z30 K above Tc) and up to ~150 K in Bi2223 (z40 K above Tc). For instance, in the slightly doped YBCO single crystal investigated by us Tc ¼ 49.2 K and T01 ¼ 85.2 K [53]. This means that the interval, in which s0 (T) is described by the ﬂuctuation theories, that is where the phase stiffness of the order parameter is maintained, DTﬂ z 36 K, is in good agreement with the aforementioned results. In the considered optimally doped single crystal, all temperature intervals, in which s0 (T) can be described by the ﬂuctuation theories, are exceptionally narrow. In particular, DTﬂ ¼ T01 TG ¼ 92.54 K 91.09 K ¼ 1.45 K. This is in good agreement with the theory, namely the higher Tc, the narrower the 935 range of SC ﬂuctuations [10,11,27]. In addition, the analogous result follows from the analysis of the temperature dependence of the pseudogap D*(T) (Figs. 6 and 7), where we have succeeded to distinctly observe a peculiarity corresponding to T01 at all values of the applied pressure, as detailed next. 3.3. Analysis of the pseudogap temperature dependence Since the excess conductivity s0 (T), equation (1), is believed to appear due to PG formation [4,9,11], it has to contain information about the PG. To deduce this information, one evidently needs an equation which describes s0 (T) over the whole temperature range Tc < T < T* and contains the PG parameter D* in the explicit form. The equation for s0 (T) accounting for the LP formation in HTSCs at T T* reads [4,9]. exp DT e2 A4 1 TT qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s’ ðεÞ ¼ : ð16Zxc ð0Þ 2εc0 sinhð2ε εc0 Þ (6) Here (1 T/T*) stands for the number of pairs formed at T < T*, while (exp(D*/T)) takes into account the number of pairs broken by ﬂuctuations when T approaches Tc. Solving equation (6) with respect to the parameter D*, which describes the pseudogap, one gets e2 A4 1 TT ﬃ: qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ D ðTÞ ¼ Tln s’ ðTÞ16Zxc ð0Þ 2εc0 sinh 2ε εc0 (7) where s0 (T) is the excess conductivity measured in experiment. In both equations T is the given temperature and T* is the pseudogap opening temperature determined from the resistivity measurements (Fig. 1). xc(0) is the coherence length along the c-axis, which is determined by the 2D-3D crossover temperature T0 from the temperature dependence of the ﬂuctuation conductivity (Fig. 3). In this way, for the determination of D*(T) one has to deﬁne from experiment the theoretical parameter εc0 and the scaling coefﬁcient A4. This is easily accomplished in the framework of the LP model [4,9], as detailed next. Fig. 4. Fluctuation conductivity lns0 as a function of lnε (symbols) of the YBa2Cu3O6.94 single crystal at P ¼ 0 GPa plotted in the whole temperature range from T* down to mf Tc . Dashed curve 1 d equation (6) with the parameters detailed in the text. Inset: ln(1/s0 ) versus ε which is linear between εc01 ¼ 0.06 and εc02 ¼ 0.09. The corresponding lnεc01 x 2.81 and lnεc02 x 2.44 are marked by the arrows in the main panel. The slope of the linear part a* ¼ 0.65 determines the parameter εc0 ¼ 1=a ¼ 0.154. 936 A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 It turned out [72] that in cuprates, in the temperature range εc01 < ε < εc02 (Tc01 < T < Tc02) the value s0 1 ∝ exp(ε), that is the dependence ln(s0 1) on ε is linear (inset to Fig. 4). The parameter εc0 ¼ 1=a ¼ 0:154 [4,9,72] is determined from the slope of the straight line a* ¼ 6.5. To calculate A4, one has to plot the lns0 (lnε) in the whole range from T* to Tcmf , as shown in Fig. 4 (symbols) for P ¼ 0 GPa. Then, using equation (6) with the already found parameters one calculates the dependences lns0 (lnε). Finally, by varying A4 the calculated curve has to be ﬁtted to the experimental data lns0 (lnε) in the range of 3D AL ﬂuctuations near Tc [4,9] (Fig. 4, dashed line), where it is assumed that D*(Tc) ¼ D(0) [28,73]. For this one also has to know the value of D*(Tc) in equation (6). In order to ﬁnd D*(T) one has to plot the experimental lns0 versus 1/T [9,74] [Fig. 5(a) and (b), symbols] and to ﬁt them to lns0 (1/T) calculated by equation (6), Fig. 5, solid curves. With this procedure the shape of the curves determined by equation (6) turns out very sensitive to the D*(Tc) value. As it follows from the ﬁgure, the best ﬁt ensues at D* ¼ 2D*(Tc)/kBTc ¼ 5 (P ¼ 0 GPa) and D* ¼ 5.8 (P ¼ 0.95 GPa) that points to the strong coupling limit. This result appears reasonable, taking into account the fact that the sample is optimally doped with a very high Tc ~ 91.1 K. One can also see that the pressure enhances the value of D* by 16%, in agreement with Refs. [25,26] reported the enhancement of the SC gap D and the ratio 2D(0)/kBTc under pressure. One more distinctive feature of the optimally doped samples with respect to the slightly doped single crystals is that equation (6) poorly describes the experimental values of s0 (T) above T0 (Fig. 4). However, should one substitute in equation (6) the D*(T) data reported in Fig. 6 instead of the D*(Tc) values, equation (6) will describe the experiment very well. When all the parameters required are found, one can plot the dependences D*(T) for all values of P. Curve 1 in Fig. 6 displays the dependence D*(T) obtained within the LP model by equation (7) at P ¼ 0 GPa with the following parameters deduced from the mf experiment: T* ¼ 141 K, Tc ¼ 91:08 K, xc(0) ¼ 0.334 Å, εc0 ¼ 0:154, and A4 ¼ 4.7. The respective dependence obtained at P ¼ 0.95 GPa is shown in Fig. 6 by open squares (curve 2). It is plotted with the parameters T* ¼ 135.7 K, Tcmf ¼ 91:83 K, xc(0) ¼ 0.405 Å, εc0 ¼ 0:147, and A4 ¼ 12. The corresponding dependences for P ¼ 0.25 GPa and 0.65 GPa are between these two curves but not shown to for the sake of data readability. The respective parameters obtained within the LP model analysis at P ¼ 0.25 GPa and 0.65 GPa are summarized in Table 1. It is worth to note that, as well as in slightly doped YBCO single crystals [53], there is a peculiarity in the sample pressure behavior at P z 6.5 GPa. This peculiarity is seen in Fig. 5. Fluctuation conductivity s0 as a function of the 1/T of YBa2Cu3O6.94 single crystal at P ¼ 0 GPa (full circles) and P ¼ 0.95 GPa (open squares). Dashed curves d calculation by equation (6) with the parameters detailed in the text. Fig. 6. Temperature dependences of the pseudogap D*(T) in the YBa2Cu3O6.94 single crystal at P ¼ 0 GPa (curve 1) and P ¼ 0.95 GPa (curve 2) calculated within the local pair model by equation (7) with the parameters detailed in the text. Solid curves are guides for the eye. the pressure dependence of d01 and xc(0), as well as of εc0 , D*, D*(TG) and Tpair, whereas r(T) and Tc smoothly vary with pressure. Fig. 6 shows that pressure noticeably increases D* at a rate dlnD*/dP z 0.32. Simultaneously, the ratio D* ¼ 2D*(Tc)/kBTc also increases by 16%, whereas the shape of the D*(T) curve is modiﬁed only slightly. Indeed, independently of pressure, the pseudogap D*(T) sharply increases in the range T* > T > Tpair demonstrating maximum at Tpair x 129 K (P ¼ 0 GPa), which is very close to Tpair z 130 K being typical for high-quality YBCO thin ﬁlms with different oxygen concentrations [9,75]. Tpair corresponds to the temperature, at which LPs transform from SBBs into FCPs [4,9], as mentioned above. Below Tpair the dependence D*(T) becomes linear with a positive slope a1 z 0.53, which appears to be pressureindependent. However, as well as in slightly doped YBCO single crystals [53], Tpair somewhat decreases under pressure down to z122 K at P ¼ 0.95 GPa, see Fig. 6. Regardless of the P value, linearity is maintained down to z100 K. A feeble maximum at T z 96 K is likely caused by a feature of the studied sample, namely, by the peculiarity in r(T) at T z 96 K, which is also seen as a minimum in the dependence lns0 (lnε) at lnε z 2.6 (Fig. 3). mf Independently of pressure, below T01 down to TG Tc a sudden * growth of the pseudogap D (T) takes place, which is distinctly observed for the ﬁrst time. This is the third non-trivial result reported in this work. Such a behavior is most likely stipulated by a transition of the sample into the range of SC ﬂuctuations, refer to Fig. 3. The speciﬁc character of the HTSCs behavior, as mentioned above, consists in the that the wave function phase stiffness of the superconductor is maintained just up to T01 [27,71]. This means that the superﬂuid density, ns, maintains a nonzero value above Tc up to T01, i.e., the ﬂuctuating pairs below T01 behave like conventional SC pairs [27,71,76]. However, in contrast to slightly doped YBCO single crystals [52], where the interval of SC ﬂuctuations DTﬂ ¼ T01 TG z 36 K, that is in line with the results of Refs. [71,76], in the case of OD single crystals DTﬂ ¼ T01 TG ¼ (92.54 91.09) K ¼ 1.45 K (P ¼ 0 GPa) and DTﬂ ¼ 1.34 K (P ¼ 0.95 GPa), that is exceptionally narrow. Nevertheless, this result is in agreement with the phase diagram of HTSCs (see Refs. [1,10] and references therein), namely, the higher the charge carrier density nf in the sample, the higher Tc and the lower T*, and, as one can see now, the narrower the range of the SC ﬂuctuations above Tc. In any case, the character of the D*(T) dependence markedly changes at T ¼ T01 most likely due to the dramatic change of the LP interaction in the sample at this temperature. A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 Fig. 7. Temperature dependence of the pseudogap D*(T) in the optimally doped YBa2Cu3O6.94 single crystal at P ¼ 0 GPa (symbols) at T < T01. Solid curve is guide for the eye. The growth of D*(T) at T < T01 is presented in Fig. 7 in detail (P ¼ 0 GPa). One sees that similarly to slightly doped YBCO single crystals [53], D*(T) rapidly increases at T < T01, has a maximum near T0 and a minimum at TG, below which there is a transition to the range of critical ﬂuctuations [9], and the ﬂuctuation theories fail. In this way, one can conclude that the transition to the SC state in both, slightly doped (SD) and optimally doped (OD) YBCO single crystals, occurs in identical way. The only exception is the disappearance of the maximum between T0 and TG in the OD single crystals at ~1 GPa. However, one should emphasize two additional essentially distinctive features. In SD single crystals the range of SC ﬂuctuations is very broad (DTﬂ z 36 K) whereas the increase D*(T) ¼ D*(TG) D*(T01) z 5 K (P ¼ 0 GPa) is rather small [52]. It is worth to emphasize that a similar increase of D* near Tc is observed for many different HTSCs including HoBCO single crystals [52] and FeAs-based superconductors [77]. This fact suggests that this increase of PG below T01 is most likely a typical feature of the HTSCs behavior just before the SC transition. The speciﬁc character of the OD single crystals consists in the fact that the increase D*(T) ¼ D*(TG) D*(T01) z 80 K at P ¼ 0 GPa is very large but occurs in the exceptionally narrow temperature interval DTﬂ z 1.5 K (Figs. 6 and 7). Such s pronounced increase of D*(T) at T < T01 is likely stipulated by a rapid increase of the number of coherent FCPs (short-range phase correlations) below T01. This conclusion can be conﬁrmed by the results of frequency-dependent complex conductivity s(u) measurements on slightly doped Bi2Sr2CaCu2O8þd (BSCCO) ﬁlms with Tc z 74 K [71]. Below Tc, the conductivity measures the phasestiffness energy kBTq directly, viz., sðuÞ ¼ isQ ðkB Tq =huÞ; (8) where sQ ≡ e2/hd is the quantum conductivity of a stack of planar conductors with the interlayer spacing d. It was shown [71] that s(u) ∝ Tq persists up to T01 z 100 K, more than 25 K above Tc, suggesting the expected presence of the short-range phase correlations in HTSCs well above Tc. In optimally doped YBCO samples the density of the charge carries nf is at least a factor of 3 larger than in SD single crystals with Tc z 49 K [6,8,58,59]. Accordingly, the density of superconducting carriers, ns, and, consequently, the density of forming FCPs (short-range phase correlations) above Tc should also be noticeably larger, that can explain the observed marked increase of D* at T < T01 in this case. Besides, the very short x(T) obtained for the OD samples is likely to promote the forming of the FCPs correlation. It should also be noted that the absolute value of D*(TG) z 230 K (Figs. 6 and 7) is a factor of 2 larger than in the SD 937 single crystals. Finally, it has to be emphasized that increase of D* observed in OD YBCO under pressure is a factor of 1.12 less than that found for SD single crystals [53]. Note that just the same result demonstrates the resistivity, namely, the decrease of r is also a factor of 1.12 less than in the SD samples. Thus, one may conclude that both effects are based on the same physical principle which can be accounted for in terms of the electron-phonon interaction. As convincingly shown in Ref. [25], a noticeable increase of both, the SC gap D(0) and the ratio 2D(0)/kBTc with pressure, observed in slightly doped polycrystals Bi2223, is accompanied by a marked decrease of the phonon spectrum frequencies in the superconductor. In this way, it is likely that the observed phonon spectrum softening is the primary cause for the increase of both, the SC gap [25,26] and the pseudogap D* ([53] and this paper) under pressure. Softening of the phonon spectrum should also lead to a reduction of the resistivity of cuprates under pressure, as observed in experiments [44,45,52,53]. It is important, as our study has revealed, that this effect does practically not depend on the HTSC doping level. At the same time, the dependence Tc(P) is strongly sensitive to the doping level suggesting another pressure effect on Tc. The increase of Tc with pressure is most likely due to the mentioned above redistribution of the charge carrier density nf, resulting in the increase of nf in the conducting CuO2 planes. As it has been mentioned above, this process is likely to take place easier in lightly doped cuprates [42,44,52,53], where dTc/dP z þ(4 5) K GPa1 [26,46,53]. Thus, one may conclude that in optimally doped samples, pressure weakly affects nf, which in optimally doped YBCO is close to saturation. Accordingly, in this case dTc/dP z þ0.7 K GPa1, that is Tc practically does not depend on pressure. 4. Conclusion The effect of the hydrostatic pressure up to 0.95 GPa on the excess conductivity s0 (T) and the pseudogap D*(T) of optimally doped YBa2Cu3O6.94 single crystals with Tc z 91.1 K at P ¼ 0 GPa has been studied. For the ﬁrst time, it was observed that the ratio D* ¼ 2D*(Tc)/kBTc as well as the pseudogap D* increase at a rate dlnD*/dP ¼ 0.32, that is only a factor of 1.12 less than in lightly doped single crystals, implying almost similar inﬂuence of pressure on the coupling strength both in OD and SD YBCO. At the same time, the pressure effect on Tc, which is believed to be due to the rearrangement of the charge carrier density nf in the conducting CuO2 planes, is minor, namely, dTc/dP z þ0.73 K GPa1. One can therefore conclude that in optimally doped samples pressure feebly inﬂuences the charge carriers density nf in the CuO2 planes, which in optimally doped YBCO is close to saturation. In consequence of this, Tc is nearly independent of pressure. However, dlnr/ dP z (17 ± 0.2) is found, which is of the same order of magnitude z(19 ± 0.2) GPa1 as in SD YBCO single crystals. Hence, the decrease of r is not related to nf, but is likely to occur in consequence of phonon spectrum softening in cuprates under pressure, that also explains the observed increase of both, D* and D*(T) with increasing pressure. In this, a certain role can also be played by other speciﬁc mechanisms of the quasiparticle scattering [78e85] stipulated by the presence of the structural and the kinematic anisotropy in the system. Independently of pressure, near Tc, s0 (T) is described well within the framework of the 3D-AL and 2D-HL ﬂuctuation theories with the MT contribution, demonstrating a 3D-2D crossover with increasing temperature. From the LP model analysis a rather peculiar temperature dependence of the pseudogap D*(T) for the OD YBCO single crystal at pressures from P ¼ 0 GPa to P ¼ 0.95 GPa was found for the ﬁrst time. The observed peculiarities allow one to comprehend better the way of the system behavior in the 938 A.L. Solovjov et al. / Current Applied Physics 16 (2016) 931e938 temperature range preceding the transition to the SC state. All these features can reasonably be accounted for in terms of the change of the local pair interaction with decreasing temperature. At the same time, independently of pressure, the resistivity curves only demonstrate a smooth decrease of r(T) below T* without any noticeable features. This result suggests that the excess conductivity contains information about PG which can be deduced using our LP model approach. Thus, the analysis performed within the model, assuming the appearance of incoherent pairs (local pairs) in high-Tc superconductors at T T*, has allowed us to get rather reasonable and self-consistent results for the temperature dependence of the pseudogap. At the same time, the pairing mechanism, which is responsible for the LP formation at such high temperatures, still remains controversial. References [1] Y. Ando, S. Komiya, K. Segawa, S. Ono, Y. Kurita, Phys. Rev. Lett. 93 (2004) 267001. [2] T. Timusk, B. Statt, Rep. Prog. Phys. 62 (1) (1999) 61. [3] J.L. Tallon, F. Barber, J.G. Storey, J.W. Loram, Phys. Rev. B 87 (2013) 140508. [4] A.L. Solovjov, M.A. Tkachenko, Metalloﬁz. Noveishie Tekhnol. 35 (2013) 19. [5] K.H. Bennemann, J.B. Katterson (Eds.), The Physics of Superconductors. Conventional and High-Tc Superconductors, Springer, New York, 2003. [6] Y. Iye, Transport Properties of High Tc Cuprates. Physical Properties of HighTemperature Superconductors, World Scientic, Singapore, 1992. [7] C.P. Slichter, Experimental Evidence for Spin Fluctuations in High Temperature Superconductors, Addison-Wesley, Redwood City, 1994. [8] J.F. Annet, N. Goldenfeld, A.J. Leggett, Phys. Properties of High-temp. Superconductors, World Scientiﬁc, Singapore, 1995, pp. 375e462. Ch. Transport properties of high-Tc cuprates. [9] A.L. Solovjov, Pseudogap and Local Pairs in High-Tc Superconductors, InTech, Rijeka, 2012, pp. 137e170. Ch. 7. [10] L. Taillefer, Ann. Rev. Condens. Matter Phys. 1 (1) (2010) 51e70. [11] A.A. Kordyuk, Low Temp. Phys. 41 (2015) 319. [12] R. Peters, J. Bauer, Phys. Rev. B 92 (2015) 014511. [13] N.F. Mott, Metal-insulator Transitions, Mir, Moscow, 1990. [14] A.M. Gabovich, A.I. Voitenko, Phys. Rev. B 80 (2009) 224501. [15] Norman, Novel Superﬂuids, vol. 2, Oxford University Press, 2013. [16] C. Berthod, Y. Fasano, I. Maggio-Aprile, A. Piriou, E. Giannini, G. Levy de Castro, O. Fischer, Phys. Rev. B 88 (2013) 014528. [17] A.A. Abrikosov, Phys. Rev. B 64 (2001) 104521. [18] L. Benfatto, S.G. Sharapov, Low Temp. Phys. 32 (6) (2006) 533e545. [19] T. Sakai, Y. Takahashi, J. Phys. Soc. Jpn. 70 (2001) 272. [20] B.P. Stojkovic-acute, D. Pines, Phys. Rev. B 55 (1997) 8576e8595. [21] K.W. Wong, W.Y. Ching, Physica C 416 (2004) 47e67. [22] S. Dzhumanov, O.K. Ganiev, S.S. Djumanov, Physica B 440 (2014) 17e32. [23] E.G. Maksimov, Usp. Fiz. Nauk. 170 (2000) 1033. [24] E.E. Zubov, Physica C 497 (2014) 67e76. [25] A.I. Dyachenko, V.Y. Tarenkov, Phys. Technol. High Press. 24 (2014) 24. [26] A. Maisuradze, A. Shengelaya, A. Amato, E. Pomjakushina, H. Keller, Phys. Rev. B 84 (2011) 184523. [27] V.J. Emery, S.A. Kivelson, Nature 374 (1995) 434e437. [28] J. Stajic, A. Iyengar, K. Levin, B.R. Boyce, T.R. Lemberger, Phys. Rev. B 68 (2003) 024520. [29] A.S. Alexandrov, V.N. Zavaritsky, S. Dzhumanov, Phys. Rev. B 69 (2004) 052505. [30] A.C. Bodi, R. Laiho, E. Lahderanta, Physica C 411 (34) (2004) 107e113. [31] V. Mishra, U. Chatterjee, J.C. Campuzano, M.R. Norman, Nat. Phys. 10 (2014) 357e360. de Melo, Phys. Rev. B 55 (1997) [32] J.R. Engelbrecht, M. Randeria, C.A.R. Sa 15153e15156. [33] V.M. Loktev, Low Temp. Phys. 22 (1996) 488. [34] O. Tchernyshyov, Phys. Rev. B 56 (1997) 3372e3380. [35] J. Sugawara, H. Iwasaki, N. Kobayashi, H. Yamane, T. Hirai, Phys. Rev. B 46 (1992) 14818e14822. [36] K. Winzer, G. Kumm, Z. Phys. B 82 (3) (1991) 317e321. [37] V.P. Gusynin, V.M. Loktev, S.G. Sharapov, JETP Lett. 65 (1997) 170. [38] L.G. Aslamasov, A.I. Larkin, Phys. Lett. A 26 (6) (1968) 238e239. [39] S. Hikami, A. Larkin, Mod. Phys. Lett. B 02 (05) (1988) 693e698. [40] J. Bardeen, L.N. Cooper, J.R. Schrieffer, Phys. Rev. 106 (1957) 162e164. [41] T. Kondo, A.D. Palczewski, Y. Hamaya, T. Takeuchi, J.S. Wen, Z.J. Xu, G. Gu, A. Kaminski, Phys. Rev. Lett. 111 (2013) 157003. [42] C.W. Chu, P.H. Hor, R.L. Meng, L. Gao, Z.J. Huang, Y.Q. Wang, Phys. Rev. Lett. 58 (1987) 405e407. [43] Y. Fang, D. Yazici, B.D. White, M.B. Maple, Phys. Rev. B 92 (2015) 094507. [44] H.J. Liu, Q. Wang, G.A. Saunders, D.P. Almond, B. Chapman, K. Kitahama, Phys. Rev. B 51 (1995) 9167e9179. [45] Q. Wang, G.A. Saunders, H.J. Liu, M.S. Acres, D.P. Almond, Phys. Rev. B 55 (1997) 8529e8543. [46] L.M. Ferreira, P. Pureur, H.A. Borges, P. Lejay, Phys. Rev. B 69 (2004) 212505. [47] M. Asta, D. de Fontaine, G. Ceder, E. Salomons, M. Kraitchman, J. Less Comm. Met. 168 (1) (1991) 39e51. [48] M. Imada, A. Fujimori, Y. Tokura, Rev. Mod. Phys. 70 (1998) 1039e1263. [49] L.J. Shen, C.C. Lam, J.Q. Li, J. Feng, Y.S. Chen, H.M. Shao, Supercond. Sci. Technol. 11 (11) (1998) 1277. [50] H.A. Borges, M.A. Continentino, Solid State Comm. 80 (3) (1991) 197e199. [51] E.V.L. De Mello, M.T.D. Orlando, J.L. Gonz alez, E.S. Caixeiro, E. Baggio-Saitovich, Phys. Rev. B 66 (2002) 092504. [52] A. Solovjov, M. Tkachenko, R. Vovk, A. Chroneos, Physica C 501 (0) (2014) 24e31. [53] A.L. Solovjov, L.V. Omelchenko, R.V. Vovk, O.V. Dobrovolskiy, D.M. Sergeyev, Z.F. Nazyrov, S.N. Kamchatnaya, Phys. B. 493 (2016) 58e67. [54] B.N. Goshchitskii, V.L. Kozhevnikov, M.V. Sadovskii, Int. J. Mod. Phys. B 2 (1988) 1331. [55] R.V. Vovk, M.A. Obolenskii, A.V. Bondarenko, I.L. Goulatis, A.V. Samoilov, A. Chroneos, V.M.P. Simoes, J. Alloys Compd. 464 (1e2) (2008) 58e66. [56] R.V. Vovk, M.A. Obolenskii, A.A. Zavgorodniy, I.L. Goulatis, V.I. Beletskii, A. Chroneos, Physica C 469 (5e6) (2009) 203e206. [57] R.V. Vovk, Z.F. Nazyrov, M.A. Obolenskii, I.L. Goulatis, A. Chroneos, V.M. Pinto Simoes, Philos. Mag. 91 (17) (2011) 2291e2302. [58] A.L. Solovjov, H.-U. Habermeier, T. Haage, Low Temp. Phys. 28 (1) (2002) 17e24. [59] A.L. Solovjov, H.-U. Habermeier, T. Haage, Low Temp. Phys. 28 (2) (2002) 99e108. [60] T. Ito, K. Takenaka, S. Uchida, Phys. Rev. Lett. 70 (1993) 3995e3998. €uerle, Phys. Rev. B 49 (1994) [61] W. Lang, G. Heine, P. Schwab, X.Z. Wang, D. Ba 4209e4217. [62] R. Haussmann, Phys. Rev. B 49 (1994) 12975e12983. [63] P.G. De Gennes, Superconductivity of Metals and Alloys, W. A. Benjamin, INC., New York - Amsterdam, 1966. [64] V.L. Ginzburg, L.D. Landau, J. Exp. Theor. Phys. 20 (1950) 1064. [65] E.M. Lifshitz, L.P. Pitaevski, Statistical Physics, vol. 2, Nauka, , Moscow, 1978. [66] B. Oh, K. Char, A.D. Kent, M. Naito, M.R. Beasley, T.H. Geballe, R.H. Hammond, A. Kapitulnik, J.M. Graybeal, Phys. Rev. B 37 (1988) 7861e7864. [67] A. Kapitulnik, M.R. Beasley, C. Castellani, C. Di Castro, Phys. Rev. B 37 (1988) 537e540. [68] T. Schneider, J.M. Singer, Phase Transition Approach to High Temperature Superconductivity: Universal Properties of Cuprate Superconductors, Imperial College Press, London, 2000. [69] Y.B. Xie, Phys. Rev. B 46 (1992) 13997e14000. [70] Y. Yamada, K. Anagawa, T. Shibauchi, T. Fujii, T. Watanabe, A. Matsuda, M. Suzuki, Phys. Rev. B 68 (2003) 054533. [71] J. Corson, R. Mallozzi, J. Orenstein, J.N. Eckstein, I. Bozovic, Nature 398 (1999) 221e223. fossez, J. Dumont, J. Lesueur, J.P. Contour, Phys. Rev. Lett. 87 [72] B. Leridon, A. De (2001) 197007. [73] R.-H. He, M. Hashimoto, H. Karapetyan, J.D. Koralek, J.P. Hinton, J.P. Testaud, V. Nathan, Y. Yoshida, H. Yao, K. Tanaka, W. Meevasana, R.G. Moore, D.H. Lu, S.-K. Mo, M. Ishikado, H. Eisaki, Z. Hussain, T.P. Devereaux, S.A. Kivelson, J. Orenstein, A. Kapitulnik, Z.-X. Shen, Science 331 (6024) (2011) 1579e1583. [74] D.D. Prokof’ev, M.P. Volkov, Y.A. Boikov, Fiz. Tverd. Tela 45 (2003) 1168e1176. [75] A.L. Solovjov, V.M. Dmitriev, Low Temp. Phys. 32 (2) (2006) 99e108. [76] A.I. Dyachenko, V.Y. Tarenkov, S.L. Sidorov, V.N. Varyukhin, A.L. Soloviev, Low Temp. Phys. 39 (4) (2013) 323e328. [77] A.L. Solovjov, M.A. Tkachenko, R.V. Vovk, M.A. Obolenskii, Low Temp. Phys. 37 (2011) 840. [78] V.M. Apalkov, M.E. Portnoi, Phys. Rev. B 65 (2002) 125310. [79] A.V. Bondarenko, V.A. Shklovskij, R.V. Vovk, M.A. Obolenskii, A.A. Prodan, Low Temp. Phys. 23 (12) (1997) 962e967. [80] D.H.S. Smith, R.V. Vovk, C.D.H. Williams, A.F.G. Wyatt, Phys. Rev. B 72 (2005) 054506. [81] V.N. Golovach, M.E. Portnoi, Phys. Rev. B 74 (2006) 085321. [82] R.V. Vovk, C.D.H. Williams, A.F.G. Wyatt, Phys. Rev. B 69 (2004), 144524e1e10. [83] D.H.S. Smith, R.V. Vovk, C.D.H. Williams, A.F.G. Wyatt, New J. Phys. 8 (8) (2006), 128e1e8. [84] P.J. Curran, V.V. Khotkevych, S.J. Bending, A.S. Gibbs, S.L. Lee, A.P. Mackenzie, Phys. Rev. B 84 (2011) 104507. [85] I.N. Adamenko, K.E. Nemchenko, V.I. Tsyganok, A.I. Chervanev, Low Temp. Phys. 20 (7) (1994) 498e504.